LMucko/crystallography-open-database huggingface dataset:
Halite-sylvite thermoelasticity Sample: als4k40, T = 600 C, P = 0.0 kbar, cell volume = 227.50 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003236
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als4k40, T = 600 C, P = 0.0 kbar, cell volume = 227.50 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1046
_cell_length_b                   6.1046
_cell_length_c                   6.1046
_cell_volume                     227.495
_cell_formula_units_Z            4
_database_code_amcsd             0003325
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    1.894
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003236
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r54382, T = 600 C, P = 14.1 kbar, cell volume = 206.91 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003237
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54382, T = 600 C, P = 14.1 kbar, cell volume = 206.91 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.9146
_cell_length_b                   5.9146
_cell_length_c                   5.9146
_cell_volume                     206.907
_cell_formula_units_Z            4
_database_code_amcsd             0003326
_diffrn_ambient_pressure         1.41e+06
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    2.083
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003237
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r54414, T = 600 C, P = 14.1 kbar, cell volume = 206.65 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003238
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54414, T = 600 C, P = 14.1 kbar, cell volume = 206.65 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.9121
_cell_length_b                   5.9121
_cell_length_c                   5.9121
_cell_volume                     206.645
_cell_formula_units_Z            4
_database_code_amcsd             0003327
_diffrn_ambient_pressure         1.41e+06
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    2.086
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003238
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r54426, T = 600 C, P = 14.1 kbar, cell volume = 206.51 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003239
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54426, T = 600 C, P = 14.1 kbar, cell volume = 206.51 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.9108
_cell_length_b                   5.9108
_cell_length_c                   5.9108
_cell_volume                     206.509
_cell_formula_units_Z            4
_database_code_amcsd             0003328
_diffrn_ambient_pressure         1.41e+06
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    2.087
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003239
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r53017, T = 600 C, P = 18.4 kbar, cell volume = 203.54 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003240
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53017, T = 600 C, P = 18.4 kbar, cell volume = 203.54 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.8823
_cell_length_b                   5.8823
_cell_length_c                   5.8823
_cell_volume                     203.536
_cell_formula_units_Z            4
_database_code_amcsd             0003329
_diffrn_ambient_pressure         1.84e+06
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    2.117
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003240
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r54482, T = 600 C, P = 20.4 kbar, cell volume = 201.21 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003241
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54482, T = 600 C, P = 20.4 kbar, cell volume = 201.21 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.8598
_cell_length_b                   5.8598
_cell_length_c                   5.8598
_cell_volume                     201.209
_cell_formula_units_Z            4
_database_code_amcsd             0003330
_diffrn_ambient_pressure         2.04e+06
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    2.142
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003241
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r54470, T = 600 C, P = 21.2 kbar, cell volume = 199.98 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003242
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54470, T = 600 C, P = 21.2 kbar, cell volume = 199.98 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.8478
_cell_length_b                   5.8478
_cell_length_c                   5.8478
_cell_volume                     199.976
_cell_formula_units_Z            4
_database_code_amcsd             0003331
_diffrn_ambient_pressure         2.12e+06
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    2.155
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003242
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r53021, T = 625 C, P = 18.3 kbar, cell volume = 203.74 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003243
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53021, T = 625 C, P = 18.3 kbar, cell volume = 203.74 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.8843
_cell_length_b                   5.8843
_cell_length_c                   5.8843
_cell_volume                     203.744
_cell_formula_units_Z            4
_database_code_amcsd             0003332
_diffrn_ambient_pressure         1.83e+06
_diffrn_ambient_temperature      898.15
_exptl_crystal_density_diffrn    2.115
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003243
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: als3k40, T = 650 C, P = 0.0 kbar, cell volume = 229.94 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003244
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als3k40, T = 650 C, P = 0.0 kbar, cell volume = 229.94 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1264
_cell_length_b                   6.1264
_cell_length_c                   6.1264
_cell_volume                     229.941
_cell_formula_units_Z            4
_database_code_amcsd             0003333
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    1.874
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003244
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r57068, T = 650 C, P = 11.5 kbar, cell volume = 215.04 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003245
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r57068, T = 650 C, P = 11.5 kbar, cell volume = 215.04 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.9911
_cell_length_b                   5.9911
_cell_length_c                   5.9911
_cell_volume                     215.040
_cell_formula_units_Z            4
_database_code_amcsd             0003334
_diffrn_ambient_pressure         1.15e+06
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    2.004
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003245
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r54366, T = 650 C, P = 15.9 kbar, cell volume = 206.67 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003246
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54366, T = 650 C, P = 15.9 kbar, cell volume = 206.67 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.9123
_cell_length_b                   5.9123
_cell_length_c                   5.9123
_cell_volume                     206.666
_cell_formula_units_Z            4
_database_code_amcsd             0003335
_diffrn_ambient_pressure         1.59e+06
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    2.085
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003246
Halite-sylvite thermoelasticity Sample: r53025, T = 650 C, P = 18.2 kbar, cell volume = 204.53 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003247
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53025, T = 650 C, P = 18.2 kbar, cell volume = 204.53 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.8919
_cell_length_b                   5.8919
_cell_length_c                   5.8919
_cell_volume                     204.534
_cell_formula_units_Z            4
_database_code_amcsd             0003336
_diffrn_ambient_pressure         1.82e+06
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    2.107
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003247
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r57136, T = 650 C, P = 19.6 kbar, cell volume = 205.26 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003248
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r57136, T = 650 C, P = 19.6 kbar, cell volume = 205.26 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.8989
_cell_length_b                   5.8989
_cell_length_c                   5.8989
_cell_volume                     205.264
_cell_formula_units_Z            4
_database_code_amcsd             0003337
_diffrn_ambient_pressure         1.96e+06
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    2.100
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003248
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r57196, T = 650 C, P = 25.2 kbar, cell volume = 200.74 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003249
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r57196, T = 650 C, P = 25.2 kbar, cell volume = 200.74 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.8552
_cell_length_b                   5.8552
_cell_length_c                   5.8552
_cell_volume                     200.736
_cell_formula_units_Z            4
_database_code_amcsd             0003338
_diffrn_ambient_pressure         2.52e+06
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    2.147
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003249
Halite-sylvite thermoelasticity Sample: r53029, T = 675 C, P = 18.1 kbar, cell volume = 204.90 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003250
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53029, T = 675 C, P = 18.1 kbar, cell volume = 204.90 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.8954
_cell_length_b                   5.8954
_cell_length_c                   5.8954
_cell_volume                     204.899
_cell_formula_units_Z            4
_database_code_amcsd             0003339
_diffrn_ambient_pressure         1.81e+06
_diffrn_ambient_temperature      948.15
_exptl_crystal_density_diffrn    2.103
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003250
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r57064, T = 700 C, P = 12.5 kbar, cell volume = 215.58 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003251
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r57064, T = 700 C, P = 12.5 kbar, cell volume = 215.58 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.9961
_cell_length_b                   5.9961
_cell_length_c                   5.9961
_cell_volume                     215.579
_cell_formula_units_Z            4
_database_code_amcsd             0003340
_diffrn_ambient_pressure         1.25e+06
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    1.999
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003251
_amcsd_formula_title             (K.4Na.6)Cl
Halite-sylvite thermoelasticity Sample: r54370, T = 700 C, P = 16.0 kbar, cell volume = 207.86 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003252
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54370, T = 700 C, P = 16.0 kbar, cell volume = 207.86 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.4Na.6)Cl
_chemical_formula_sum            'Cl K0.4 Na0.6'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.9237
_cell_length_b                   5.9237
_cell_length_c                   5.9237
_cell_volume                     207.864
_cell_formula_units_Z            4
_database_code_amcsd             0003341
_diffrn_ambient_pressure         1.6e+06
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    2.073
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.4 Na.6) Cl'
_cod_database_code               9003252